Self-assembly of 3-D 4d?4f coordination frameworks based on 1-D inorganic heterometallic chains and linear organic linkers
Gu, Xiaojun; Xue, Dongfeng; CrystEngComm 9 (2007) 471–; doi:10.1039/b704544a

data_7202893
_publ_section_title
;
 Self-assembly of 3-D 4d?4f coordination frameworks based on 1-D
 inorganic heterometallic chains and linear organic linkers
;
_journal_issue                   6
_journal_name_full               CrystEngComm
_journal_page_first              471
_journal_paper_doi               10.1039/b704544a
_journal_volume                  9
_journal_year                    2007
_chemical_formula_sum            'C17 H9.5 Ag Eu N2.5 O9'
_chemical_formula_weight         652.60
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                100.486(3)
_cell_angle_beta                 101.062(3)
_cell_angle_gamma                95.619(3)
_cell_formula_units_Z            2
_cell_length_a                   7.2636(18)
_cell_length_b                   10.409(3)
_cell_length_c                   11.639(3)
_cell_measurement_temperature    293(2)
_cell_volume                     841.1(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.971
_diffrn_measured_fraction_theta_max 0.971
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0119
_diffrn_reflns_av_sigmaI/netI    0.0241
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            4682
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         1.82
_exptl_absorpt_coefficient_mu    4.923
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.577
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             622
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.02
_refine_diff_density_max         3.633
_refine_diff_density_min         -2.252
_refine_diff_density_rms         0.160
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.053
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     284
_refine_ls_number_reflns         3334
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.053
_refine_ls_R_factor_all          0.0319
_refine_ls_R_factor_gt           0.0308
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0369P)^2^+6.4592P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0787
_refine_ls_wR_factor_ref         0.0794
_reflns_number_gt                3204
_reflns_number_total             3334
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b704544a.txt
_cod_data_source_block           2
_cod_original_sg_symbol_H-M      P-1
_cod_original_formula_sum        'C17 H9.50 Ag Eu N2.50 O9'
_cod_database_code               7202893